 
data_shelx
 
_audit_creation_method            'SHELXL-2016/4'
_shelx_SHELXL_version_number      '2016/4'
_chemical_name_systematic         ?
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          
   'O9 S2, Ca0.08 H4 O2, 2(O4 S), 1.92(Ca), 4(Na)'
_chemical_formula_sum
 'Ca2 H4 Na4 O19 S4' 
_chemical_formula_weight          608.39

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na'  'Na'   0.0362   0.0249
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ca'  'Ca'   0.2262   0.3064
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'S'  'S'   0.1246   0.1234
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H'  'H'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       monoclinic
_space_group_IT_number            11
_space_group_name_H-M_alt         'P 21/m'
_space_group_name_Hall            '-P 2yb'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _symmetry_equiv_pos_as_xyz
 'x, y, z'
 '-x, y+1/2, -z'
 '-x, -y, -z'
 'x, -y-1/2, z'
 
_cell_length_a                    6.4596(4)
_cell_length_b                    6.8703(5)
_cell_length_c                    9.4685(7)
_cell_angle_alpha                 90
_cell_angle_beta                  104.580(4)
_cell_angle_gamma                 90
_cell_volume                      406.67(5)
_cell_formula_units_Z             1
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used     2751
_cell_measurement_theta_min       3.26
_cell_measurement_theta_max       26.72
 
_exptl_crystal_description        'prism'
_exptl_crystal_colour             'colourless'
_exptl_crystal_density_meas       ?
_exptl_crystal_density_method     ?
_exptl_crystal_density_diffrn     2.484          
_exptl_crystal_F_000              304
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?
_exptl_crystal_size_max           0.24
_exptl_crystal_size_mid           0.07
_exptl_crystal_size_min           0.06
_exptl_absorpt_coefficient_mu     1.424
_shelx_estimated_absorpt_T_min    ?
_shelx_estimated_absorpt_T_max    ?
_exptl_absorpt_correction_type    'multi-scan'
_exptl_absorpt_correction_T_min   0.6265
_exptl_absorpt_correction_T_max   0.7460
_exptl_absorpt_process_details    'Bruker SADABS'
_exptl_absorpt_special_details    ?
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_source                    'fine-focus sealed tube'  
_diffrn_measurement_device_type   'PHOTON 100 CMOS'
_diffrn_measurement_method        'φ and ω scans'
_diffrn_detector_area_resol_mean  ?
_diffrn_reflns_number             7865
_diffrn_reflns_av_unetI/netI      0.0646
_diffrn_reflns_av_R_equivalents   0.0848
_diffrn_reflns_limit_h_min        -8
_diffrn_reflns_limit_h_max        8
_diffrn_reflns_limit_k_min        -9
_diffrn_reflns_limit_k_max        9
_diffrn_reflns_limit_l_min        -12
_diffrn_reflns_limit_l_max        12
_diffrn_reflns_theta_min          2.222
_diffrn_reflns_theta_max          28.977
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.982
_diffrn_measured_fraction_theta_full  0.991
_diffrn_reflns_Laue_measured_fraction_max    0.982
_diffrn_reflns_Laue_measured_fraction_full   0.991
_diffrn_reflns_point_group_measured_fraction_max   0.982
_diffrn_reflns_point_group_measured_fraction_full  0.991
_reflns_number_total              1143
_reflns_number_gt                 793
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection        'Bruker APEX3'
_computing_cell_refinement        'Bruker SAINT'
_computing_data_reduction         'Bruker SAINT'
_computing_structure_solution     'Superflip (Palatinus & Chapuis, 2007)'
_computing_structure_refinement   'SHELXL-2016/4 (Sheldrick, 2016)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
_refine_special_details           ?
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0667P)²+1.4637P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
_atom_sites_solution_hydrogens    difmap
_refine_ls_hydrogen_treatment     refxyz
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        .
_refine_ls_number_reflns          1143
_refine_ls_number_parameters      103
_refine_ls_number_restraints      1
_refine_ls_R_factor_all           0.0982
_refine_ls_R_factor_gt            0.0571
_refine_ls_wR_factor_ref          0.1444
_refine_ls_wR_factor_gt           0.1277
_refine_ls_goodness_of_fit_ref    1.045
_refine_ls_restrained_S_all       1.045
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
NA1 Na 0.1500(6) 0.0042(3) 0.8020(3) 0.0677(10) Uani 1 1 d . . . . .
CA1 Ca 0.3397(2) 0.250000 0.45448(15) 0.0179(3) Uani 1 2 d S T P . .
S1 S 0.8372(2) 0.250000 0.49442(16) 0.0100(3) Uani 1 2 d S T P . .
S2A S 0.3085(7) 0.250000 0.1262(4) 0.0177(8) Uani 0.5 2 d S T P . .
S2B S 0.1932(7) 0.250000 0.1106(4) 0.0171(8) Uani 0.5 2 d S T P . .
O1 O 0.9563(7) 0.250000 0.3812(5) 0.0192(10) Uani 1 2 d S T P . .
O2 O 0.9872(7) 0.250000 0.6380(5) 0.0225(10) Uani 1 2 d S T P . .
O3 O 0.6955(4) 0.0782(4) 0.4745(3) 0.0179(7) Uani 1 1 d . . . . .
O4 O 0.2634(6) 0.0787(5) 0.2070(4) 0.0342(9) Uani 1 1 d . . . . .
O5A O 0.1687(19) 0.250000 -0.0196(11) 0.022(2) Uani 0.5 2 d S T P . .
O5B O 0.290(2) 0.250000 -0.0149(13) 0.031(3) Uani 0.5 2 d S T P . .
O6A O 0.5319(15) 0.250000 0.1186(12) 0.031(2) Uani 0.5 2 d S T P . .
O6B O -0.0329(19) 0.250000 0.0613(13) 0.062(4) Uani 0.5 2 d S T P . .
OW1 O 0.4833(8) 0.250000 0.7188(6) 0.0332(13) Uani 1 2 d DS T P . .
OW2 O -0.2695(17) 0.250000 0.0518(11) 0.031(2) Uani 0.5 2 d S T P . .
H1 H 0.571(8) 0.146(7) 0.767(6) 0.037 Uiso 1 1 d D U . . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
NA1 OW2 2.242(7) 3_556 ?
NA1 O2 2.355(4) 1_455 ?
NA1 O5A 2.370(8) 1_556 ?
NA1 O6B 2.407(9) 3_556 ?
NA1 O5B 2.426(9) 1_556 ?
NA1 O1 2.435(4) 3_656 ?
NA1 O6A 2.657(8) 3_656 ?
NA1 O4 2.711(5) 3_556 ?
NA1 OW1 2.994(6) . ?
NA1 O3 3.079(4) 3_656 ?
NA1 S2B 3.094(5) 3_556 ?
NA1 S1 3.324(3) 3_656 ?
CA1 O3 2.380(3) 2_656 ?
CA1 O3 2.380(3) 3_656 ?
CA1 O1 2.398(4) 1_455 ?
CA1 OW1 2.440(5) . ?
CA1 O3 2.549(3) . ?
CA1 O3 2.549(3) 4_565 ?
CA1 O4 2.557(4) . ?
CA1 O4 2.557(4) 4_565 ?
CA1 S2A 3.063(4) . ?
CA1 S1 3.1402(18) . ?
CA1 S2B 3.154(4) . ?
CA1 O2 3.193(5) 1_455 ?
S1 O2 1.457(5) . ?
S1 O1 1.468(5) . ?
S1 O3 1.476(3) . ?
S1 O3 1.476(3) 4_565 ?
S1 NA1 3.324(3) 3_656 ?
S1 NA1 3.324(3) 2_656 ?
S1 CA1 3.3608(18) 1_655 ?
S1 OW1 3.490(6) . ?
S2A S2B 0.722(4) . ?
S2A O5B 1.312(12) . ?
S2A O5A 1.447(11) . ?
S2A O6A 1.463(11) . ?
S2A O4 1.472(4) . ?
S2A O4 1.472(4) 4_565 ?
S2A O6B 2.135(13) . ?
S2A OW2 2.983(11) 1_655 ?
S2B O5A 1.203(11) . ?
S2B O6B 1.417(13) . ?
S2B O5B 1.475(12) . ?
S2B O4 1.488(4) . ?
S2B O4 1.488(4) 4_565 ?
S2B O6A 2.170(11) . ?
S2B OW2 2.899(11) . ?
S2B NA1 3.094(5) 3_556 ?
S2B NA1 3.094(5) 2_556 ?
S2B O1 3.298(6) 1_455 ?
O1 O2 2.389(6) . ?
O1 CA1 2.398(4) 1_655 ?
O1 O3 2.400(5) . ?
O1 O3 2.400(5) 4_565 ?
O1 NA1 2.435(4) 3_656 ?
O1 NA1 2.435(4) 2_656 ?
O1 O6B 3.047(13) 1_655 ?
O1 OW2 3.093(11) 1_655 ?
O1 O4 3.113(5) 4_665 ?
O1 O4 3.113(5) 1_655 ?
O1 O6A 3.204(11) . ?
O2 NA1 2.355(4) 4_665 ?
O2 NA1 2.355(4) 1_655 ?
O2 O3 2.423(5) . ?
O2 O3 2.423(5) 4_565 ?
O2 OW1 3.102(7) 1_655 ?
O2 O5A 3.158(11) 1_656 ?
O2 CA1 3.193(5) 1_655 ?
O2 O4 3.327(5) 3_656 ?
O2 O4 3.327(5) 2_656 ?
O2 O5B 3.374(13) 1_656 ?
O3 O3 2.361(6) 4_565 ?
O3 CA1 2.380(3) 3_656 ?
O3 O3 2.895(6) 3_656 ?
O3 OW1 2.950(4) 3_656 ?
O3 NA1 3.079(4) 3_656 ?
O3 O4 3.151(4) 3_656 ?
O3 OW1 3.197(6) . ?
O3 O1 3.235(4) 3_756 ?
O4 O4 2.354(7) 4_565 ?
O4 O6B 2.371(10) . ?
O4 O5A 2.388(9) . ?
O4 O6A 2.414(9) . ?
O4 O5B 2.452(11) . ?
O4 NA1 2.711(5) 3_556 ?
O4 OW1 2.773(5) 3_656 ?
O4 O1 3.113(5) 1_455 ?
O4 O3 3.151(4) 3_656 ?
O5A O5B 0.772(12) . ?
O5A O6B 1.669(18) . ?
O5A NA1 2.370(8) 1_554 ?
O5A NA1 2.370(8) 4_564 ?
O5A O6A 2.381(15) . ?
O5A O4 2.388(9) 4_565 ?
O5A OW2 3.071(16) . ?
O5A O2 3.158(11) 1_454 ?
O5A OW2 3.520(16) 1_655 ?
O5B O6A 1.746(16) . ?
O5B O6B 2.372(18) . ?
O5B NA1 2.426(9) 1_554 ?
O5B NA1 2.426(9) 4_564 ?
O5B O4 2.452(11) 4_565 ?
O5B OW2 2.756(15) 1_655 ?
O5B OW1 3.083(13) 1_554 ?
O5B O2 3.374(13) 1_454 ?
O6A OW2 1.567(14) 1_655 ?
O6A O4 2.414(9) 4_565 ?
O6A NA1 2.657(8) 2_656 ?
O6A NA1 2.657(8) 3_656 ?
O6A O6B 2.994(15) 1_655 ?
O6B OW2 1.508(16) . ?
O6B O4 2.371(10) 4_565 ?
O6B NA1 2.407(9) 2_556 ?
O6B NA1 2.407(9) 3_556 ?
O6B O6A 2.994(15) 1_455 ?
O6B O1 3.047(13) 1_455 ?
O6B NA1 3.426(11) 1_554 ?
OW1 H1 0.95(4) . ?
OW1 O4 2.773(5) 2_656 ?
OW1 O4 2.773(5) 3_656 ?
OW1 O3 2.950(4) 3_656 ?
OW1 O3 2.950(4) 2_656 ?
OW1 NA1 2.994(6) 4_565 ?
OW1 O5B 3.083(13) 1_556 ?
OW1 O2 3.102(7) 1_455 ?
OW1 OW2 3.155(11) 1_656 ?
OW1 O3 3.197(6) 4_565 ?
OW1 H1 0.95(4) . ?
OW2 O6A 1.567(14) 1_455 ?
OW2 NA1 2.242(7) 2_556 ?
OW2 NA1 2.242(7) 3_556 ?
OW2 O5B 2.756(15) 1_455 ?
OW2 S2A 2.983(11) 1_455 ?
OW2 O1 3.093(11) 1_455 ?
OW2 OW1 3.155(11) 1_454 ?
OW2 O4 3.339(8) 3 ?
OW2 O4 3.339(8) 2 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
OW2 NA1 O2 173.2(3) 3_556 1_455 ?
OW2 NA1 O5A 99.6(3) 3_556 1_556 ?
O2 NA1 O5A 83.9(2) 1_455 1_556 ?
OW2 NA1 O6B 37.7(4) 3_556 3_556 ?
O2 NA1 O6B 136.6(3) 1_455 3_556 ?
O5A NA1 O6B 95.8(3) 1_556 3_556 ?
OW2 NA1 O5B 95.3(3) 3_556 1_556 ?
O2 NA1 O5B 89.8(2) 1_455 1_556 ?
O5A NA1 O5B 18.5(3) 1_556 1_556 ?
O6B NA1 O5B 103.4(3) 3_556 1_556 ?
OW2 NA1 O1 82.7(2) 3_556 3_656 ?
O2 NA1 O1 92.61(13) 1_455 3_656 ?
O5A NA1 O1 166.7(4) 1_556 3_656 ?
O6B NA1 O1 78.0(3) 3_556 3_656 ?
O5B NA1 O1 174.7(3) 1_556 3_656 ?
OW2 NA1 O6A 36.1(3) 3_556 3_656 ?
O2 NA1 O6A 147.5(3) 1_455 3_656 ?
O5A NA1 O6A 111.7(3) 1_556 3_656 ?
O6B NA1 O6A 72.3(3) 3_556 3_656 ?
O5B NA1 O6A 97.7(3) 1_556 3_656 ?
O1 NA1 O6A 77.8(2) 3_656 3_656 ?
OW2 NA1 O4 92.2(3) 3_556 3_556 ?
O2 NA1 O4 81.77(16) 1_455 3_556 ?
O5A NA1 O4 92.6(3) 1_556 3_556 ?
O6B NA1 O4 54.8(3) 3_556 3_556 ?
O5B NA1 O4 110.8(3) 1_556 3_556 ?
O1 NA1 O4 74.22(14) 3_656 3_556 ?
O6A NA1 O4 123.79(19) 3_656 3_556 ?
OW2 NA1 OW1 116.3(3) 3_556 . ?
O2 NA1 OW1 69.73(15) 1_455 . ?
O5A NA1 OW1 82.8(3) 1_556 . ?
O6B NA1 OW1 153.6(3) 3_556 . ?
O5B NA1 OW1 68.4(3) 1_556 . ?
O1 NA1 OW1 108.04(16) 3_656 . ?
O6A NA1 OW1 83.6(2) 3_656 . ?
O4 NA1 OW1 151.44(14) 3_556 . ?
OW2 NA1 O3 104.3(3) 3_556 3_656 ?
O2 NA1 O3 75.99(14) 1_455 3_656 ?
O5A NA1 O3 140.1(3) 1_556 3_656 ?
O6B NA1 O3 122.5(2) 3_556 3_656 ?
O5B NA1 O3 126.4(3) 1_556 3_656 ?
O1 NA1 O3 49.94(12) 3_656 3_656 ?
O6A NA1 O3 74.2(2) 3_656 3_656 ?
O4 NA1 O3 117.53(12) 3_556 3_656 ?
OW1 NA1 O3 58.10(12) . 3_656 ?
OW2 NA1 S2B 63.5(3) 3_556 3_556 ?
O2 NA1 S2B 110.47(18) 1_455 3_556 ?
O5A NA1 S2B 97.1(3) 1_556 3_556 ?
O6B NA1 S2B 26.2(3) 3_556 3_556 ?
O5B NA1 S2B 111.4(3) 1_556 3_556 ?
O1 NA1 S2B 72.13(13) 3_656 3_556 ?
O6A NA1 S2B 96.22(18) 3_656 3_556 ?
O4 NA1 S2B 28.75(10) 3_556 3_556 ?
OW1 NA1 S2B 179.74(16) . 3_556 ?
O3 NA1 S2B 122.07(10) 3_656 3_556 ?
OW2 NA1 S1 92.0(2) 3_556 3_656 ?
O2 NA1 S1 85.53(11) 1_455 3_656 ?
O5A NA1 S1 165.6(2) 1_556 3_656 ?
O6B NA1 S1 98.7(2) 3_556 3_656 ?
O5B NA1 S1 152.3(3) 1_556 3_656 ?
O1 NA1 S1 23.71(10) 3_656 3_656 ?
O6A NA1 S1 73.3(2) 3_656 3_656 ?
O4 NA1 S1 95.56(10) 3_556 3_656 ?
OW1 NA1 S1 84.37(12) . 3_656 ?
O3 NA1 S1 26.31(6) 3_656 3_656 ?
S2B NA1 S1 95.80(9) 3_556 3_656 ?
O3 CA1 O3 142.64(15) 2_656 3_656 ?
O3 CA1 O1 85.21(8) 2_656 1_455 ?
O3 CA1 O1 85.21(8) 3_656 1_455 ?
O3 CA1 OW1 75.46(8) 2_656 . ?
O3 CA1 OW1 75.46(8) 3_656 . ?
O1 CA1 OW1 113.28(18) 1_455 . ?
O3 CA1 O3 124.50(8) 2_656 . ?
O3 CA1 O3 71.86(11) 3_656 . ?
O1 CA1 O3 150.24(8) 1_455 . ?
OW1 CA1 O3 79.67(14) . . ?
O3 CA1 O3 71.86(11) 2_656 4_565 ?
O3 CA1 O3 124.50(8) 3_656 4_565 ?
O1 CA1 O3 150.24(8) 1_455 4_565 ?
OW1 CA1 O3 79.67(14) . 4_565 ?
O3 CA1 O3 55.19(13) . 4_565 ?
O3 CA1 O4 133.23(11) 2_656 . ?
O3 CA1 O4 79.22(11) 3_656 . ?
O1 CA1 O4 77.76(13) 1_455 . ?
OW1 CA1 O4 151.12(9) . . ?
O3 CA1 O4 79.46(11) . . ?
O3 CA1 O4 104.09(12) 4_565 . ?
O3 CA1 O4 79.21(11) 2_656 4_565 ?
O3 CA1 O4 133.23(11) 3_656 4_565 ?
O1 CA1 O4 77.76(13) 1_455 4_565 ?
OW1 CA1 O4 151.12(9) . 4_565 ?
O3 CA1 O4 104.09(12) . 4_565 ?
O3 CA1 O4 79.46(11) 4_565 4_565 ?
O4 CA1 O4 54.81(15) . 4_565 ?
O3 CA1 S2A 107.47(8) 2_656 . ?
O3 CA1 S2A 107.47(8) 3_656 . ?
O1 CA1 S2A 84.66(14) 1_455 . ?
OW1 CA1 S2A 162.05(16) . . ?
O3 CA1 S2A 84.44(11) . . ?
O3 CA1 S2A 84.44(11) 4_565 . ?
O4 CA1 S2A 28.59(8) . . ?
O4 CA1 S2A 28.59(8) 4_565 . ?
O3 CA1 S1 97.68(7) 2_656 . ?
O3 CA1 S1 97.68(7) 3_656 . ?
O1 CA1 S1 170.43(12) 1_455 . ?
OW1 CA1 S1 76.29(13) . . ?
O3 CA1 S1 27.67(6) . . ?
O3 CA1 S1 27.67(6) 4_565 . ?
O4 CA1 S1 93.76(10) . . ?
O4 CA1 S1 93.76(10) 4_565 . ?
S2A CA1 S1 85.76(10) . . ?
O3 CA1 S2B 105.46(8) 2_656 . ?
O3 CA1 S2B 105.46(8) 3_656 . ?
O1 CA1 S2B 71.43(14) 1_455 . ?
OW1 CA1 S2B 175.29(16) . . ?
O3 CA1 S2B 96.16(11) . . ?
O3 CA1 S2B 96.16(11) 4_565 . ?
O4 CA1 S2B 27.78(8) . . ?
O4 CA1 S2B 27.78(8) 4_565 . ?
S2A CA1 S2B 13.23(7) . . ?
S1 CA1 S2B 98.99(9) . . ?
O3 CA1 O2 73.40(8) 2_656 1_455 ?
O3 CA1 O2 73.40(8) 3_656 1_455 ?
O1 CA1 O2 48.05(13) 1_455 1_455 ?
OW1 CA1 O2 65.24(15) . 1_455 ?
O3 CA1 O2 135.48(10) . 1_455 ?
O3 CA1 O2 135.48(10) 4_565 1_455 ?
O4 CA1 O2 119.96(12) . 1_455 ?
O4 CA1 O2 119.96(12) 4_565 1_455 ?
S2A CA1 O2 132.71(12) . 1_455 ?
S1 CA1 O2 141.53(9) . 1_455 ?
S2B CA1 O2 119.48(12) . 1_455 ?
O2 S1 O1 109.5(3) . . ?
O2 S1 O3 111.36(17) . . ?
O1 S1 O3 109.17(16) . . ?
O2 S1 O3 111.36(17) . 4_565 ?
O1 S1 O3 109.17(16) . 4_565 ?
O3 S1 O3 106.2(2) . 4_565 ?
O2 S1 CA1 122.2(2) . . ?
O1 S1 CA1 128.34(19) . . ?
O3 S1 CA1 53.27(12) . . ?
O3 S1 CA1 53.27(12) 4_565 . ?
O2 S1 NA1 129.48(16) . 3_656 ?
O1 S1 NA1 41.81(12) . 3_656 ?
O3 S1 NA1 67.56(14) . 3_656 ?
O3 S1 NA1 117.29(15) 4_565 3_656 ?
CA1 S1 NA1 98.07(7) . 3_656 ?
O2 S1 NA1 129.48(16) . 2_656 ?
O1 S1 NA1 41.81(12) . 2_656 ?
O3 S1 NA1 117.29(15) . 2_656 ?
O3 S1 NA1 67.56(14) 4_565 2_656 ?
CA1 S1 NA1 98.07(7) . 2_656 ?
NA1 S1 NA1 63.39(9) 3_656 2_656 ?
O2 S1 CA1 70.8(2) . 1_655 ?
O1 S1 CA1 38.72(17) . 1_655 ?
O3 S1 CA1 124.80(12) . 1_655 ?
O3 S1 CA1 124.80(12) 4_565 1_655 ?
CA1 S1 CA1 167.05(7) . 1_655 ?
NA1 S1 CA1 71.04(7) 3_656 1_655 ?
NA1 S1 CA1 71.04(7) 2_656 1_655 ?
O2 S1 OW1 79.4(2) . . ?
O1 S1 OW1 171.1(2) . . ?
O3 S1 OW1 66.29(13) . . ?
O3 S1 OW1 66.29(14) 4_565 . ?
CA1 S1 OW1 42.78(9) . . ?
NA1 S1 OW1 132.30(9) 3_656 . ?
NA1 S1 OW1 132.30(9) 2_656 . ?
CA1 S1 OW1 150.17(10) 1_655 . ?
S2B S2A O5B 88.0(7) . . ?
S2B S2A O5A 56.0(6) . . ?
O5B S2A O5A 32.0(5) . . ?
S2B S2A O6A 165.8(7) . . ?
O5B S2A O6A 77.8(7) . . ?
O5A S2A O6A 109.8(7) . . ?
S2B S2A O4 77.2(4) . . ?
O5B S2A O4 123.4(3) . . ?
O5A S2A O4 109.8(4) . . ?
O6A S2A O4 110.6(3) . . ?
S2B S2A O4 77.2(4) . 4_565 ?
O5B S2A O4 123.4(3) . 4_565 ?
O5A S2A O4 109.8(4) . 4_565 ?
O6A S2A O4 110.6(3) . 4_565 ?
O4 S2A O4 106.2(4) . 4_565 ?
S2B S2A O6B 4.7(5) . . ?
O5B S2A O6B 83.3(7) . . ?
O5A S2A O6B 51.3(6) . . ?
O6A S2A O6B 161.1(6) . . ?
O4 S2A O6B 79.9(3) . . ?
O4 S2A O6B 79.9(3) 4_565 . ?
S2B S2A OW2 155.3(6) . 1_655 ?
O5B S2A OW2 67.3(6) . 1_655 ?
O5A S2A OW2 99.3(6) . 1_655 ?
O6A S2A OW2 10.5(5) . 1_655 ?
O4 S2A OW2 115.8(3) . 1_655 ?
O4 S2A OW2 115.8(3) 4_565 1_655 ?
O6B S2A OW2 150.6(4) . 1_655 ?
S2B S2A CA1 90.5(5) . . ?
O5B S2A CA1 178.5(6) . . ?
O5A S2A CA1 146.5(6) . . ?
O6A S2A CA1 103.7(5) . . ?
O4 S2A CA1 56.24(18) . . ?
O4 S2A CA1 56.24(18) 4_565 . ?
O6B S2A CA1 95.3(4) . . ?
OW2 S2A CA1 114.2(2) 1_655 . ?
S2A S2B O5A 94.2(8) . . ?
S2A S2B O6B 172.9(8) . . ?
O5A S2B O6B 78.7(8) . . ?
S2A S2B O5B 62.7(7) . . ?
O5A S2B O5B 31.5(6) . . ?
O6B S2B O5B 110.2(8) . . ?
S2A S2B O4 74.6(3) . . ?
O5A S2B O4 124.7(2) . . ?
O6B S2B O4 109.4(4) . . ?
O5B S2B O4 111.6(4) . . ?
S2A S2B O4 74.6(3) . 4_565 ?
O5A S2B O4 124.7(2) . 4_565 ?
O6B S2B O4 109.4(4) . 4_565 ?
O5B S2B O4 111.6(4) . 4_565 ?
O4 S2B O4 104.5(4) . 4_565 ?
S2A S2B O6A 9.5(5) . . ?
O5A S2B O6A 84.6(7) . . ?
O6B S2B O6A 163.3(6) . . ?
O5B S2B O6A 53.2(6) . . ?
O4 S2B O6A 80.2(3) . . ?
O4 S2B O6A 80.2(3) 4_565 . ?
S2A S2B OW2 179.3(6) . . ?
O5A S2B OW2 86.6(7) . . ?
O6B S2B OW2 7.9(5) . . ?
O5B S2B OW2 118.0(6) . . ?
O4 S2B OW2 105.0(3) . . ?
O4 S2B OW2 105.0(3) 4_565 . ?
O6A S2B OW2 171.2(4) . . ?
S2A S2B NA1 135.8(3) . 3_556 ?
O5A S2B NA1 110.9(5) . 3_556 ?
O6B S2B NA1 48.7(3) . 3_556 ?
O5B S2B NA1 133.8(4) . 3_556 ?
O4 S2B NA1 61.2(2) . 3_556 ?
O4 S2B NA1 114.2(2) 4_565 3_556 ?
O6A S2B NA1 140.77(17) . 3_556 ?
OW2 S2B NA1 43.78(14) . 3_556 ?
S2A S2B NA1 135.8(3) . 2_556 ?
O5A S2B NA1 110.9(5) . 2_556 ?
O6B S2B NA1 48.7(3) . 2_556 ?
O5B S2B NA1 133.8(4) . 2_556 ?
O4 S2B NA1 114.2(2) . 2_556 ?
O4 S2B NA1 61.2(2) 4_565 2_556 ?
O6A S2B NA1 140.77(17) . 2_556 ?
OW2 S2B NA1 43.78(14) . 2_556 ?
NA1 S2B NA1 68.73(14) 3_556 2_556 ?
S2A S2B CA1 76.2(5) . . ?
O5A S2B CA1 170.4(7) . . ?
O6B S2B CA1 110.9(5) . . ?
O5B S2B CA1 138.9(6) . . ?
O4 S2B CA1 53.21(18) . . ?
O4 S2B CA1 53.21(18) 4_565 . ?
O6A S2B CA1 85.8(3) . . ?
OW2 S2B CA1 103.0(2) . . ?
NA1 S2B CA1 76.87(9) 3_556 . ?
NA1 S2B CA1 76.87(9) 2_556 . ?
S2A S2B O1 119.8(5) . 1_455 ?
O5A S2B O1 146.0(7) . 1_455 ?
O6B S2B O1 67.3(5) . 1_455 ?
O5B S2B O1 177.5(6) . 1_455 ?
O4 S2B O1 69.7(2) . 1_455 ?
O4 S2B O1 69.7(2) 4_565 1_455 ?
O6A S2B O1 129.3(3) . 1_455 ?
OW2 S2B O1 59.5(2) . 1_455 ?
NA1 S2B O1 44.64(8) 3_556 1_455 ?
NA1 S2B O1 44.64(8) 2_556 1_455 ?
CA1 S2B O1 43.56(9) . 1_455 ?
S1 O1 O2 35.09(16) . . ?
S1 O1 CA1 118.8(2) . 1_655 ?
O2 O1 CA1 83.68(18) . 1_655 ?
S1 O1 O3 35.53(11) . . ?
O2 O1 O3 60.78(15) . . ?
CA1 O1 O3 131.51(17) 1_655 . ?
S1 O1 O3 35.53(10) . 4_565 ?
O2 O1 O3 60.78(15) . 4_565 ?
CA1 O1 O3 131.51(17) 1_655 4_565 ?
O3 O1 O3 58.93(17) . 4_565 ?
S1 O1 NA1 114.48(17) . 3_656 ?
O2 O1 NA1 131.39(11) . 3_656 ?
CA1 O1 NA1 106.96(15) 1_655 3_656 ?
O3 O1 NA1 79.11(13) . 3_656 ?
O3 O1 NA1 121.1(2) 4_565 3_656 ?
S1 O1 NA1 114.48(17) . 2_656 ?
O2 O1 NA1 131.39(11) . 2_656 ?
CA1 O1 NA1 106.96(15) 1_655 2_656 ?
O3 O1 NA1 121.1(2) . 2_656 ?
O3 O1 NA1 79.11(13) 4_565 2_656 ?
NA1 O1 NA1 91.65(19) 3_656 2_656 ?
S1 O1 O6B 150.8(3) . 1_655 ?
O2 O1 O6B 174.1(3) . 1_655 ?
CA1 O1 O6B 90.4(3) 1_655 1_655 ?
O3 O1 O6B 124.0(2) . 1_655 ?
O3 O1 O6B 124.0(2) 4_565 1_655 ?
NA1 O1 O6B 50.58(13) 3_656 1_655 ?
NA1 O1 O6B 50.58(13) 2_656 1_655 ?
S1 O1 OW2 122.4(3) . 1_655 ?
O2 O1 OW2 157.5(3) . 1_655 ?
CA1 O1 OW2 118.8(3) 1_655 1_655 ?
O3 O1 OW2 100.1(2) . 1_655 ?
O3 O1 OW2 100.1(2) 4_565 1_655 ?
NA1 O1 OW2 45.97(9) 3_656 1_655 ?
NA1 O1 OW2 45.97(9) 2_656 1_655 ?
O6B O1 OW2 28.4(3) 1_655 1_655 ?
S1 O1 O4 155.19(13) . 4_665 ?
O2 O1 O4 129.66(19) . 4_665 ?
CA1 O1 O4 53.40(11) 1_655 4_665 ?
O3 O1 O4 168.81(18) . 4_665 ?
O3 O1 O4 127.51(10) 4_565 4_665 ?
NA1 O1 O4 89.82(16) 3_656 4_665 ?
NA1 O1 O4 56.94(14) 2_656 4_665 ?
O6B O1 O4 45.3(2) 1_655 4_665 ?
OW2 O1 O4 70.6(2) 1_655 4_665 ?
S1 O1 O4 155.19(13) . 1_655 ?
O2 O1 O4 129.66(19) . 1_655 ?
CA1 O1 O4 53.40(11) 1_655 1_655 ?
O3 O1 O4 127.51(10) . 1_655 ?
O3 O1 O4 168.81(18) 4_565 1_655 ?
NA1 O1 O4 56.94(14) 3_656 1_655 ?
NA1 O1 O4 89.82(16) 2_656 1_655 ?
O6B O1 O4 45.3(2) 1_655 1_655 ?
OW2 O1 O4 70.6(2) 1_655 1_655 ?
O4 O1 O4 44.44(14) 4_665 1_655 ?
S1 O1 O6A 93.6(3) . . ?
O2 O1 O6A 128.7(3) . . ?
CA1 O1 O6A 147.6(2) 1_655 . ?
O3 O1 O6A 75.1(2) . . ?
O3 O1 O6A 75.1(2) 4_565 . ?
NA1 O1 O6A 54.16(14) 3_656 . ?
NA1 O1 O6A 54.16(14) 2_656 . ?
O6B O1 O6A 57.2(3) 1_655 . ?
OW2 O1 O6A 28.7(3) 1_655 . ?
O4 O1 O6A 97.1(2) 4_665 . ?
O4 O1 O6A 97.1(2) 1_655 . ?
S1 O2 NA1 134.17(9) . 4_665 ?
S1 O2 NA1 134.17(9) . 1_655 ?
NA1 O2 NA1 91.61(19) 4_665 1_655 ?
S1 O2 O1 35.40(17) . . ?
NA1 O2 O1 125.45(15) 4_665 . ?
NA1 O2 O1 125.45(15) 1_655 . ?
S1 O2 O3 34.58(10) . . ?
NA1 O2 O3 156.5(2) 4_665 . ?
NA1 O2 O3 102.61(10) 1_655 . ?
O1 O2 O3 59.83(15) . . ?
S1 O2 O3 34.58(10) . 4_565 ?
NA1 O2 O3 102.61(10) 4_665 4_565 ?
NA1 O2 O3 156.5(2) 1_655 4_565 ?
O1 O2 O3 59.83(15) . 4_565 ?
O3 O2 O3 58.32(17) . 4_565 ?
S1 O2 OW1 129.3(3) . 1_655 ?
NA1 O2 OW1 64.85(14) 4_665 1_655 ?
NA1 O2 OW1 64.85(14) 1_655 1_655 ?
O1 O2 OW1 93.9(2) . 1_655 ?
O3 O2 OW1 138.27(17) . 1_655 ?
O3 O2 OW1 138.27(17) 4_565 1_655 ?
S1 O2 O5A 161.0(4) . 1_656 ?
NA1 O2 O5A 48.26(12) 4_665 1_656 ?
NA1 O2 O5A 48.26(12) 1_655 1_656 ?
O1 O2 O5A 163.6(3) . 1_656 ?
O3 O2 O5A 133.2(2) . 1_656 ?
O3 O2 O5A 133.2(2) 4_565 1_656 ?
OW1 O2 O5A 69.7(3) 1_655 1_656 ?
S1 O2 CA1 83.7(2) . 1_655 ?
NA1 O2 CA1 95.58(16) 4_665 1_655 ?
NA1 O2 CA1 95.58(15) 1_655 1_655 ?
O1 O2 CA1 48.28(13) . 1_655 ?
O3 O2 CA1 101.45(16) . 1_655 ?
O3 O2 CA1 101.45(16) 4_565 1_655 ?
OW1 O2 CA1 45.58(12) 1_655 1_655 ?
O5A O2 CA1 115.3(3) 1_656 1_655 ?
S1 O2 O4 97.40(18) . 3_656 ?
NA1 O2 O4 112.45(19) 4_665 3_656 ?
NA1 O2 O4 53.75(13) 1_655 3_656 ?
O1 O2 O4 121.59(14) . 3_656 ?
O3 O2 O4 64.21(12) . 3_656 ?
O3 O2 O4 103.08(17) 4_565 3_656 ?
OW1 O2 O4 118.58(13) 1_655 3_656 ?
O5A O2 O4 69.10(19) 1_656 3_656 ?
CA1 O2 O4 137.12(8) 1_655 3_656 ?
S1 O2 O4 97.40(18) . 2_656 ?
NA1 O2 O4 53.75(13) 4_665 2_656 ?
NA1 O2 O4 112.45(19) 1_655 2_656 ?
O1 O2 O4 121.59(14) . 2_656 ?
O3 O2 O4 103.08(17) . 2_656 ?
O3 O2 O4 64.21(12) 4_565 2_656 ?
OW1 O2 O4 118.58(13) 1_655 2_656 ?
O5A O2 O4 69.10(19) 1_656 2_656 ?
CA1 O2 O4 137.12(8) 1_655 2_656 ?
O4 O2 O4 85.48(16) 3_656 2_656 ?
S1 O2 O5B 174.1(4) . 1_656 ?
NA1 O2 O5B 45.96(9) 4_665 1_656 ?
NA1 O2 O5B 45.96(9) 1_655 1_656 ?
O1 O2 O5B 150.5(3) . 1_656 ?
O3 O2 O5B 142.08(19) . 1_656 ?
O3 O2 O5B 142.08(19) 4_565 1_656 ?
OW1 O2 O5B 56.7(2) 1_655 1_656 ?
O5A O2 O5B 13.0(2) 1_656 1_656 ?
CA1 O2 O5B 102.3(2) 1_655 1_656 ?
O4 O2 O5B 78.30(18) 3_656 1_656 ?
O4 O2 O5B 78.30(18) 2_656 1_656 ?
S1 O3 O3 36.91(12) . 4_565 ?
S1 O3 CA1 145.25(18) . 3_656 ?
O3 O3 CA1 161.32(8) 4_565 3_656 ?
S1 O3 O1 35.30(12) . . ?
O3 O3 O1 60.53(8) 4_565 . ?
CA1 O3 O1 134.10(14) 3_656 . ?
S1 O3 O2 34.06(12) . . ?
O3 O3 O2 60.84(8) 4_565 . ?
CA1 O3 O2 113.28(13) 3_656 . ?
O1 O3 O2 59.39(16) . . ?
S1 O3 CA1 99.06(14) . . ?
O3 O3 CA1 62.40(6) 4_565 . ?
CA1 O3 CA1 108.14(11) 3_656 . ?
O1 O3 CA1 116.63(13) . . ?
O2 O3 CA1 111.31(14) . . ?
S1 O3 O3 144.5(2) . 3_656 ?
O3 O3 O3 111.77(11) 4_565 3_656 ?
CA1 O3 O3 56.77(10) 3_656 3_656 ?
O1 O3 O3 165.1(2) . 3_656 ?
O2 O3 O3 130.1(2) . 3_656 ?
CA1 O3 O3 51.36(9) . 3_656 ?
S1 O3 OW1 145.5(2) . 3_656 ?
O3 O3 OW1 139.84(9) 4_565 3_656 ?
CA1 O3 OW1 53.19(11) 3_656 3_656 ?
O1 O3 OW1 110.44(17) . 3_656 ?
O2 O3 OW1 152.73(17) . 3_656 ?
CA1 O3 OW1 95.90(13) . 3_656 ?
O3 O3 OW1 66.30(15) 3_656 3_656 ?
S1 O3 NA1 86.14(15) . 3_656 ?
O3 O3 NA1 100.59(7) 4_565 3_656 ?
CA1 O3 NA1 98.08(11) 3_656 3_656 ?
O1 O3 NA1 50.95(11) . 3_656 ?
O2 O3 NA1 105.46(16) . 3_656 ?
CA1 O3 NA1 120.07(13) . 3_656 ?
O3 O3 NA1 123.82(16) 3_656 3_656 ?
OW1 O3 NA1 59.49(13) 3_656 3_656 ?
S1 O3 O4 104.54(17) . 3_656 ?
O3 O3 O4 110.00(8) 4_565 3_656 ?
CA1 O3 O4 52.88(9) 3_656 3_656 ?
O1 O3 O4 128.53(17) . 3_656 ?
O2 O3 O4 71.96(14) . 3_656 ?
CA1 O3 O4 94.97(12) . 3_656 ?
O3 O3 O4 65.18(13) 3_656 3_656 ?
OW1 O3 O4 104.95(14) 3_656 3_656 ?
NA1 O3 O4 141.61(13) 3_656 3_656 ?
S1 O3 OW1 88.69(15) . . ?
O3 O3 OW1 68.33(6) 4_565 . ?
CA1 O3 OW1 93.24(10) 3_656 . ?
O1 O3 OW1 123.58(13) . . ?
O2 O3 OW1 76.34(16) . . ?
CA1 O3 OW1 48.67(11) . . ?
O3 O3 OW1 57.67(12) 3_656 . ?
OW1 O3 OW1 123.97(12) 3_656 . ?
NA1 O3 OW1 166.56(13) 3_656 . ?
O4 O3 OW1 51.81(10) 3_656 . ?
S1 O3 O1 99.24(14) . 3_756 ?
O3 O3 O1 134.19(7) 4_565 3_756 ?
CA1 O3 O1 47.63(8) 3_656 3_756 ?
O1 O3 O1 91.18(11) . 3_756 ?
O2 O3 O1 73.95(10) . 3_756 ?
CA1 O3 O1 150.76(14) . 3_756 ?
O3 O3 O1 102.36(15) 3_656 3_756 ?
OW1 O3 O1 81.46(12) 3_656 3_756 ?
NA1 O3 O1 83.77(12) 3_656 3_756 ?
O4 O3 O1 58.34(11) 3_656 3_756 ?
OW1 O3 O1 109.33(14) . 3_756 ?
S2A O4 S2B 28.22(16) . . ?
S2A O4 O4 36.90(18) . 4_565 ?
S2B O4 O4 37.74(18) . 4_565 ?
S2A O4 O6B 62.4(3) . . ?
S2B O4 O6B 34.3(3) . . ?
O4 O4 O6B 60.23(16) 4_565 . ?
S2A O4 O5A 34.8(3) . . ?
S2B O4 O5A 24.5(2) . . ?
O4 O4 O5A 60.47(15) 4_565 . ?
O6B O4 O5A 41.1(4) . . ?
S2A O4 O6A 34.6(3) . . ?
S2B O4 O6A 62.4(3) . . ?
O4 O4 O6A 60.81(13) 4_565 . ?
O6B O4 O6A 95.8(3) . . ?
O5A O4 O6A 59.5(4) . . ?
S2A O4 O5B 26.5(2) . . ?
S2B O4 O5B 34.0(3) . . ?
O4 O4 O5B 61.31(15) 4_565 . ?
O6B O4 O5B 58.9(4) . . ?
O5A O4 O5B 18.3(3) . . ?
O6A O4 O5B 42.1(4) . . ?
S2A O4 CA1 95.2(2) . . ?
S2B O4 CA1 99.0(2) . . ?
O4 O4 CA1 62.59(8) 4_565 . ?
O6B O4 CA1 104.2(3) . . ?
O5A O4 CA1 122.90(19) . . ?
O6A O4 CA1 96.0(3) . . ?
O5B O4 CA1 121.7(2) . . ?
S2A O4 NA1 118.3(3) . 3_556 ?
S2B O4 NA1 90.1(3) . 3_556 ?
O4 O4 NA1 102.13(9) 4_565 3_556 ?
O6B O4 NA1 56.1(3) . 3_556 ?
O5A O4 NA1 92.8(3) . 3_556 ?
O6A O4 NA1 151.6(3) . 3_556 ?
O5B O4 NA1 110.8(3) . 3_556 ?
CA1 O4 NA1 94.96(13) . 3_556 ?
S2A O4 OW1 127.0(3) . 3_656 ?
S2B O4 OW1 150.3(3) . 3_656 ?
O4 O4 OW1 144.51(12) 4_565 3_656 ?
O6B O4 OW1 152.9(2) . 3_656 ?
O5A O4 OW1 129.1(3) . 3_656 ?
O6A O4 OW1 93.2(2) . 3_656 ?
O5B O4 OW1 116.4(3) . 3_656 ?
CA1 O4 OW1 100.20(16) . 3_656 ?
NA1 O4 OW1 110.52(16) 3_556 3_656 ?
S2A O4 O1 102.0(2) . 1_455 ?
S2B O4 O1 83.6(2) . 1_455 ?
O4 O4 O1 67.78(7) 4_565 1_455 ?
O6B O4 O1 65.9(3) . 1_455 ?
O5A O4 O1 103.7(3) . 1_455 ?
O6A O4 O1 127.51(18) . 1_455 ?
O5B O4 O1 117.6(2) . 1_455 ?
CA1 O4 O1 48.84(10) . 1_455 ?
NA1 O4 O1 48.84(10) 3_556 1_455 ?
OW1 O4 O1 125.98(17) 3_656 1_455 ?
S2A O4 O3 142.2(2) . 3_656 ?
S2B O4 O3 142.8(2) . 3_656 ?
O4 O4 O3 110.00(8) 4_565 3_656 ?
O6B O4 O3 126.0(3) . 3_656 ?
O5A O4 O3 165.8(3) . 3_656 ?
O6A O4 O3 127.2(3) . 3_656 ?
O5B O4 O3 167.8(3) . 3_656 ?
CA1 O4 O3 47.91(8) . 3_656 ?
NA1 O4 O3 78.64(11) 3_556 3_656 ?
OW1 O4 O3 64.95(14) 3_656 3_656 ?
O1 O4 O3 62.18(11) 1_455 3_656 ?
O5B O5A S2B 94.1(15) . . ?
O5B O5A S2A 64.3(13) . . ?
S2B O5A S2A 29.8(3) . . ?
O5B O5A O6B 150.4(17) . . ?
S2B O5A O6B 56.3(7) . . ?
S2A O5A O6B 86.2(7) . . ?
O5B O5A NA1 84.8(10) . 1_554 ?
S2B O5A NA1 134.47(19) . 1_554 ?
S2A O5A NA1 126.0(4) . 1_554 ?
O6B O5A NA1 114.9(5) . 1_554 ?
O5B O5A NA1 84.8(10) . 4_564 ?
S2B O5A NA1 134.47(19) . 4_564 ?
S2A O5A NA1 126.0(4) . 4_564 ?
O6B O5A NA1 114.9(5) . 4_564 ?
NA1 O5A NA1 90.9(4) 1_554 4_564 ?
O5B O5A O6A 28.9(12) . . ?
S2B O5A O6A 65.2(6) . . ?
S2A O5A O6A 35.3(4) . . ?
O6B O5A O6A 121.5(7) . . ?
NA1 O5A O6A 105.0(4) 1_554 . ?
NA1 O5A O6A 105.0(4) 4_564 . ?
O5B O5A O4 85.5(12) . . ?
S2B O5A O4 30.82(18) . . ?
S2A O5A O4 35.5(2) . . ?
O6B O5A O4 68.9(5) . . ?
NA1 O5A O4 104.17(13) 1_554 . ?
NA1 O5A O4 161.3(4) 4_564 . ?
O6A O5A O4 60.8(3) . . ?
O5B O5A O4 85.5(12) . 4_565 ?
S2B O5A O4 30.82(18) . 4_565 ?
S2A O5A O4 35.5(2) . 4_565 ?
O6B O5A O4 68.9(5) . 4_565 ?
NA1 O5A O4 161.3(4) 1_554 4_565 ?
NA1 O5A O4 104.17(13) 4_564 4_565 ?
O6A O5A O4 60.8(3) . 4_565 ?
O4 O5A O4 59.1(3) . 4_565 ?
O5B O5A OW2 164.5(15) . . ?
S2B O5A OW2 70.4(6) . . ?
S2A O5A OW2 100.2(6) . . ?
O6B O5A OW2 14.1(5) . . ?
NA1 O5A OW2 105.8(4) 1_554 . ?
NA1 O5A OW2 105.8(4) 4_564 . ?
O6A O5A OW2 135.6(5) . . ?
O4 O5A OW2 81.0(4) . . ?
O4 O5A OW2 81.0(4) 4_565 . ?
O5B O5A O2 99.7(15) . 1_454 ?
S2B O5A O2 166.2(8) . 1_454 ?
S2A O5A O2 163.9(8) . 1_454 ?
O6B O5A O2 109.9(6) . 1_454 ?
NA1 O5A O2 47.87(19) 1_554 1_454 ?
NA1 O5A O2 47.87(19) 4_564 1_454 ?
O6A O5A O2 128.6(5) . 1_454 ?
O4 O5A O2 150.15(16) . 1_454 ?
O4 O5A O2 150.15(16) 4_565 1_454 ?
OW2 O5A O2 95.8(4) . 1_454 ?
O5B O5A OW2 7.5(12) . 1_655 ?
S2B O5A OW2 86.6(6) . 1_655 ?
S2A O5A OW2 56.7(5) . 1_655 ?
O6B O5A OW2 142.9(7) . 1_655 ?
NA1 O5A OW2 90.1(4) 1_554 1_655 ?
NA1 O5A OW2 90.1(4) 4_564 1_655 ?
O6A O5A OW2 21.4(3) . 1_655 ?
O4 O5A OW2 79.0(3) . 1_655 ?
O4 O5A OW2 79.0(3) 4_565 1_655 ?
OW2 O5A OW2 157.0(5) . 1_655 ?
O2 O5A OW2 107.2(4) 1_454 1_655 ?
O5A O5B S2A 83.7(14) . . ?
O5A O5B S2B 54.4(12) . . ?
S2A O5B S2B 29.3(3) . . ?
O5A O5B O6A 138.7(17) . . ?
S2A O5B O6A 55.0(6) . . ?
S2B O5B O6A 84.3(7) . . ?
O5A O5B O6B 20.3(12) . . ?
S2A O5B O6B 63.4(6) . . ?
S2B O5B O6B 34.1(4) . . ?
O6A O5B O6B 118.4(7) . . ?
O5A O5B NA1 76.7(10) . 1_554 ?
S2A O5B NA1 130.6(4) . 1_554 ?
S2B O5B NA1 114.8(5) . 1_554 ?
O6A O5B NA1 128.5(4) . 1_554 ?
O6B O5B NA1 91.1(4) . 1_554 ?
O5A O5B NA1 76.7(10) . 4_564 ?
S2A O5B NA1 130.6(4) . 4_564 ?
S2B O5B NA1 114.8(5) . 4_564 ?
O6A O5B NA1 128.5(4) . 4_564 ?
O6B O5B NA1 91.1(4) . 4_564 ?
NA1 O5B NA1 88.2(4) 1_554 4_564 ?
O5A O5B O4 76.2(12) . . ?
S2A O5B O4 30.10(19) . . ?
S2B O5B O4 34.4(2) . . ?
O6A O5B O4 67.8(5) . . ?
O6B O5B O4 58.9(4) . . ?
NA1 O5B O4 100.6(2) 1_554 . ?
NA1 O5B O4 148.5(5) 4_564 . ?
O5A O5B O4 76.2(12) . 4_565 ?
S2A O5B O4 30.10(19) . 4_565 ?
S2B O5B O4 34.4(2) . 4_565 ?
O6A O5B O4 67.8(5) . 4_565 ?
O6B O5B O4 58.9(4) . 4_565 ?
NA1 O5B O4 148.5(5) 1_554 4_565 ?
NA1 O5B O4 100.6(2) 4_564 4_565 ?
O4 O5B O4 57.4(3) . 4_565 ?
O5A O5B OW2 170.4(16) . 1_655 ?
S2A O5B OW2 86.7(7) . 1_655 ?
S2B O5B OW2 115.9(7) . 1_655 ?
O6A O5B OW2 31.7(4) . 1_655 ?
O6B O5B OW2 150.0(6) . 1_655 ?
NA1 O5B OW2 109.9(4) 1_554 1_655 ?
NA1 O5B OW2 109.9(4) 4_564 1_655 ?
O4 O5B OW2 95.4(4) . 1_655 ?
O4 O5B OW2 95.4(4) 4_565 1_655 ?
O5A O5B OW1 124.5(15) . 1_554 ?
S2A O5B OW1 151.8(8) . 1_554 ?
S2B O5B OW1 178.9(8) . 1_554 ?
O6A O5B OW1 96.8(6) . 1_554 ?
O6B O5B OW1 144.8(6) . 1_554 ?
NA1 O5B OW1 64.5(3) 1_554 1_554 ?
NA1 O5B OW1 64.5(3) 4_564 1_554 ?
O4 O5B OW1 146.2(3) . 1_554 ?
O4 O5B OW1 146.2(3) 4_565 1_554 ?
OW2 O5B OW1 65.1(3) 1_655 1_554 ?
O5A O5B O2 67.3(14) . 1_454 ?
S2A O5B O2 151.0(8) . 1_454 ?
S2B O5B O2 121.7(7) . 1_454 ?
O6A O5B O2 154.0(7) . 1_454 ?
O6B O5B O2 87.6(5) . 1_454 ?
NA1 O5B O2 44.3(2) 1_554 1_454 ?
NA1 O5B O2 44.3(2) 4_564 1_454 ?
O4 O5B O2 133.3(4) . 1_454 ?
O4 O5B O2 133.3(4) 4_565 1_454 ?
OW2 O5B O2 122.3(4) 1_655 1_454 ?
OW1 O5B O2 57.2(2) 1_554 1_454 ?
S2A O6A OW2 159.7(9) . 1_655 ?
S2A O6A O5B 47.2(5) . . ?
OW2 O6A O5B 112.5(8) 1_655 . ?
S2A O6A S2B 4.7(2) . . ?
OW2 O6A S2B 155.1(8) 1_655 . ?
O5B O6A S2B 42.6(4) . . ?
S2A O6A O5A 34.9(4) . . ?
OW2 O6A O5A 124.9(7) 1_655 . ?
O5B O6A O5A 12.4(5) . . ?
S2B O6A O5A 30.2(3) . . ?
S2A O6A O4 34.8(2) . . ?
OW2 O6A O4 150.81(14) 1_655 . ?
O5B O6A O4 70.1(4) . . ?
S2B O6A O4 37.42(17) . . ?
O5A O6A O4 59.7(3) . . ?
S2A O6A O4 34.8(2) . 4_565 ?
OW2 O6A O4 150.81(14) 1_655 4_565 ?
O5B O6A O4 70.1(4) . 4_565 ?
S2B O6A O4 37.42(17) . 4_565 ?
O5A O6A O4 59.7(3) . 4_565 ?
O4 O6A O4 58.4(3) . 4_565 ?
S2A O6A NA1 133.5(3) . 2_656 ?
OW2 O6A NA1 57.4(3) 1_655 2_656 ?
O5B O6A NA1 133.8(3) . 2_656 ?
S2B O6A NA1 135.3(2) . 2_656 ?
O5A O6A NA1 137.7(2) . 2_656 ?
O4 O6A NA1 142.6(5) . 2_656 ?
O4 O6A NA1 98.8(2) 4_565 2_656 ?
S2A O6A NA1 133.5(3) . 3_656 ?
OW2 O6A NA1 57.4(3) 1_655 3_656 ?
O5B O6A NA1 133.8(3) . 3_656 ?
S2B O6A NA1 135.3(2) . 3_656 ?
O5A O6A NA1 137.7(2) . 3_656 ?
O4 O6A NA1 98.8(2) . 3_656 ?
O4 O6A NA1 142.6(5) 4_565 3_656 ?
NA1 O6A NA1 82.2(3) 2_656 3_656 ?
S2A O6A O6B 172.6(7) . 1_655 ?
OW2 O6A O6B 12.9(5) 1_655 1_655 ?
O5B O6A O6B 125.4(6) . 1_655 ?
S2B O6A O6B 168.0(5) . 1_655 ?
O5A O6A O6B 137.8(6) . 1_655 ?
O4 O6A O6B 148.5(2) . 1_655 ?
O4 O6A O6B 148.5(2) 4_565 1_655 ?
NA1 O6A O6B 50.0(2) 2_656 1_655 ?
NA1 O6A O6B 50.0(2) 3_656 1_655 ?
S2A O6A O1 128.6(6) . . ?
OW2 O6A O1 71.7(5) 1_655 . ?
O5B O6A O1 175.8(6) . . ?
S2B O6A O1 133.3(4) . . ?
O5A O6A O1 163.5(5) . . ?
O4 O6A O1 106.3(3) . . ?
O4 O6A O1 106.3(3) 4_565 . ?
NA1 O6A O1 47.99(17) 2_656 . ?
NA1 O6A O1 47.99(17) 3_656 . ?
O6B O6A O1 58.8(3) 1_655 . ?
S2A O6A O3 90.9(4) . . ?
OW2 O6A O3 108.2(6) 1_655 . ?
O5B O6A O3 134.5(5) . . ?
S2B O6A O3 95.3(3) . . ?
O5A O6A O3 123.4(4) . . ?
O4 O6A O3 64.4(2) . . ?
O4 O6A O3 84.2(3) 4_565 . ?
NA1 O6A O3 85.6(3) 2_656 . ?
NA1 O6A O3 58.5(2) 3_656 . ?
O6B O6A O3 96.1(3) 1_655 . ?
O1 O6A O3 41.88(15) . . ?
S2B O6B OW2 164.7(10) . . ?
S2B O6B O5A 45.0(5) . . ?
OW2 O6B O5A 150.3(10) . . ?
S2B O6B S2A 2.4(3) . . ?
OW2 O6B S2A 167.1(9) . . ?
O5A O6B S2A 42.6(5) . . ?
S2B O6B O4 36.3(2) . . ?
OW2 O6B O4 133.8(6) . . ?
O5A O6B O4 70.0(5) . . ?
S2A O6B O4 37.7(2) . . ?
S2B O6B O4 36.3(2) . 4_565 ?
OW2 O6B O4 133.8(6) . 4_565 ?
O5A O6B O4 70.0(5) . 4_565 ?
S2A O6B O4 37.7(2) . 4_565 ?
O4 O6B O4 59.5(3) . 4_565 ?
S2B O6B O5B 35.7(5) . . ?
OW2 O6B O5B 159.5(9) . . ?
O5A O6B O5B 9.2(5) . . ?
S2A O6B O5B 33.3(4) . . ?
O4 O6B O5B 62.3(4) . . ?
O4 O6B O5B 62.3(4) 4_565 . ?
S2B O6B NA1 105.1(5) . 2_556 ?
OW2 O6B NA1 65.2(4) . 2_556 ?
O5A O6B NA1 129.4(3) . 2_556 ?
S2A O6B NA1 106.7(4) . 2_556 ?
O4 O6B NA1 111.4(5) . 2_556 ?
O4 O6B NA1 69.1(2) 4_565 2_556 ?
O5B O6B NA1 125.7(3) . 2_556 ?
S2B O6B NA1 105.1(5) . 3_556 ?
OW2 O6B NA1 65.2(4) . 3_556 ?
O5A O6B NA1 129.4(3) . 3_556 ?
S2A O6B NA1 106.7(4) . 3_556 ?
O4 O6B NA1 69.1(2) . 3_556 ?
O4 O6B NA1 111.4(5) 4_565 3_556 ?
O5B O6B NA1 125.7(3) . 3_556 ?
NA1 O6B NA1 93.1(5) 2_556 3_556 ?
S2B O6B O6A 151.3(8) . 1_455 ?
OW2 O6B O6A 13.4(5) . 1_455 ?
O5A O6B O6A 163.7(8) . 1_455 ?
S2A O6B O6A 153.7(6) . 1_455 ?
O4 O6B O6A 123.5(5) . 1_455 ?
O4 O6B O6A 123.5(5) 4_565 1_455 ?
O5B O6B O6A 173.0(6) . 1_455 ?
NA1 O6B O6A 57.7(3) 2_556 1_455 ?
NA1 O6B O6A 57.7(3) 3_556 1_455 ?
S2B O6B O1 87.3(6) . 1_455 ?
OW2 O6B O1 77.5(6) . 1_455 ?
O5A O6B O1 132.2(7) . 1_455 ?
S2A O6B O1 89.7(4) . 1_455 ?
O4 O6B O1 68.8(3) . 1_455 ?
O4 O6B O1 68.8(3) 4_565 1_455 ?
O5B O6B O1 123.0(5) . 1_455 ?
NA1 O6B O1 51.4(2) 2_556 1_455 ?
NA1 O6B O1 51.4(2) 3_556 1_455 ?
O6A O6B O1 64.0(3) 1_455 1_455 ?
S2B O6B NA1 73.9(5) . 1_554 ?
OW2 O6B NA1 119.0(6) . 1_554 ?
O5A O6B NA1 38.8(3) . 1_554 ?
S2A O6B NA1 71.9(3) . 1_554 ?
O4 O6B NA1 78.4(3) . 1_554 ?
O4 O6B NA1 106.7(4) 4_565 1_554 ?
O5B O6B NA1 45.1(3) . 1_554 ?
NA1 O6B NA1 162.8(3) 2_556 1_554 ?
NA1 O6B NA1 103.87(14) 3_556 1_554 ?
O6A O6B NA1 129.7(3) 1_455 1_554 ?
O1 O6B NA1 144.2(2) 1_455 1_554 ?
H1 OW1 CA1 121(3) . . ?
H1 OW1 O4 104(3) . 2_656 ?
CA1 OW1 O4 107.93(16) . 2_656 ?
H1 OW1 O4 13(3) . 3_656 ?
CA1 OW1 O4 107.93(16) . 3_656 ?
O4 OW1 O4 109.0(2) 2_656 3_656 ?
H1 OW1 O3 79(3) . 3_656 ?
CA1 OW1 O3 51.35(10) . 3_656 ?
O4 OW1 O3 153.3(2) 2_656 3_656 ?
O4 OW1 O3 69.45(10) 3_656 3_656 ?
H1 OW1 O3 164(3) . 2_656 ?
CA1 OW1 O3 51.35(10) . 2_656 ?
O4 OW1 O3 69.45(10) 2_656 2_656 ?
O4 OW1 O3 153.3(2) 3_656 2_656 ?
O3 OW1 O3 99.69(19) 3_656 2_656 ?
H1 OW1 NA1 132(3) . 4_565 ?
CA1 OW1 NA1 99.03(16) . 4_565 ?
O4 OW1 NA1 83.77(12) 2_656 4_565 ?
O4 OW1 NA1 144.1(2) 3_656 4_565 ?
O3 OW1 NA1 113.52(18) 3_656 4_565 ?
O3 OW1 NA1 62.41(10) 2_656 4_565 ?
H1 OW1 NA1 80(3) . . ?
CA1 OW1 NA1 99.03(16) . . ?
O4 OW1 NA1 144.1(2) 2_656 . ?
O4 OW1 NA1 83.77(12) 3_656 . ?
O3 OW1 NA1 62.41(10) 3_656 . ?
O3 OW1 NA1 113.52(18) 2_656 . ?
NA1 OW1 NA1 68.68(16) 4_565 . ?
H1 OW1 O5B 85(3) . 1_556 ?
CA1 OW1 O5B 135.3(3) . 1_556 ?
O4 OW1 O5B 97.3(2) 2_656 1_556 ?
O4 OW1 O5B 97.3(2) 3_656 1_556 ?
O3 OW1 O5B 109.3(2) 3_656 1_556 ?
O3 OW1 O5B 109.3(2) 2_656 1_556 ?
NA1 OW1 O5B 47.02(18) 4_565 1_556 ?
NA1 OW1 O5B 47.02(18) . 1_556 ?
H1 OW1 O2 125(3) . 1_455 ?
CA1 OW1 O2 69.18(15) . 1_455 ?
O4 OW1 O2 124.72(12) 2_656 1_455 ?
O4 OW1 O2 124.72(12) 3_656 1_455 ?
O3 OW1 O2 68.16(12) 3_656 1_455 ?
O3 OW1 O2 68.16(12) 2_656 1_455 ?
NA1 OW1 O2 45.42(11) 4_565 1_455 ?
NA1 OW1 O2 45.42(11) . 1_455 ?
O5B OW1 O2 66.1(3) 1_556 1_455 ?
H1 OW1 OW2 55(3) . 1_656 ?
CA1 OW1 OW2 172.3(3) . 1_656 ?
O4 OW1 OW2 68.21(16) 2_656 1_656 ?
O4 OW1 OW2 68.21(16) 3_656 1_656 ?
O3 OW1 OW2 129.83(10) 3_656 1_656 ?
O3 OW1 OW2 129.83(10) 2_656 1_656 ?
NA1 OW1 OW2 87.3(2) 4_565 1_656 ?
NA1 OW1 OW2 87.3(2) . 1_656 ?
O5B OW1 OW2 52.4(3) 1_556 1_656 ?
O2 OW1 OW2 118.5(3) 1_455 1_656 ?
H1 OW1 O3 108(3) . 4_565 ?
CA1 OW1 O3 51.66(12) . 4_565 ?
O4 OW1 O3 63.24(12) 2_656 4_565 ?
O4 OW1 O3 98.69(18) 3_656 4_565 ?
O3 OW1 O3 90.33(15) 3_656 4_565 ?
O3 OW1 O3 56.03(12) 2_656 4_565 ?
NA1 OW1 O3 116.74(10) 4_565 4_565 ?
NA1 OW1 O3 150.07(19) . 4_565 ?
O5B OW1 O3 158.07(8) 1_556 4_565 ?
O2 OW1 O3 115.23(18) 1_455 4_565 ?
OW2 OW1 O3 121.4(2) 1_656 4_565 ?
H1 OW1 H1 0(6) . . ?
CA1 OW1 H1 121(3) . . ?
O4 OW1 H1 104(3) 2_656 . ?
O4 OW1 H1 13(3) 3_656 . ?
O3 OW1 H1 79(3) 3_656 . ?
O3 OW1 H1 164(3) 2_656 . ?
NA1 OW1 H1 132(3) 4_565 . ?
NA1 OW1 H1 80(3) . . ?
O5B OW1 H1 85(3) 1_556 . ?
O2 OW1 H1 125(3) 1_455 . ?
OW2 OW1 H1 55(3) 1_656 . ?
O3 OW1 H1 108(3) 4_565 . ?
O6B OW2 O6A 153.7(9) . 1_455 ?
O6B OW2 NA1 77.1(4) . 2_556 ?
O6A OW2 NA1 86.6(4) 1_455 2_556 ?
O6B OW2 NA1 77.1(4) . 3_556 ?
O6A OW2 NA1 86.6(4) 1_455 3_556 ?
NA1 OW2 NA1 102.4(4) 2_556 3_556 ?
O6B OW2 O5B 170.5(8) . 1_455 ?
O6A OW2 O5B 35.8(5) 1_455 1_455 ?
NA1 OW2 O5B 108.5(4) 2_556 1_455 ?
NA1 OW2 O5B 108.5(4) 3_556 1_455 ?
O6B OW2 S2B 7.4(5) . . ?
O6A OW2 S2B 146.3(7) 1_455 . ?
NA1 OW2 S2B 72.8(3) 2_556 . ?
NA1 OW2 S2B 72.8(3) 3_556 . ?
O5B OW2 S2B 177.9(5) 1_455 . ?
O6B OW2 S2A 163.4(7) . 1_455 ?
O6A OW2 S2A 9.8(4) 1_455 1_455 ?
NA1 OW2 S2A 92.7(3) 2_556 1_455 ?
NA1 OW2 S2A 92.7(3) 3_556 1_455 ?
O5B OW2 S2A 26.0(3) 1_455 1_455 ?
S2B OW2 S2A 156.1(4) . 1_455 ?
O6B OW2 O5A 15.6(5) . . ?
O6A OW2 O5A 169.3(7) 1_455 . ?
NA1 OW2 O5A 86.7(3) 2_556 . ?
NA1 OW2 O5A 86.7(3) 3_556 . ?
O5B OW2 O5A 154.9(5) 1_455 . ?
S2B OW2 O5A 23.0(2) . . ?
S2A OW2 O5A 179.1(4) 1_455 . ?
O6B OW2 O1 74.1(6) . 1_455 ?
O6A OW2 O1 79.6(6) 1_455 1_455 ?
NA1 OW2 O1 51.4(2) 2_556 1_455 ?
NA1 OW2 O1 51.4(2) 3_556 1_455 ?
O5B OW2 O1 115.4(4) 1_455 1_455 ?
S2B OW2 O1 66.7(2) . 1_455 ?
S2A OW2 O1 89.3(3) 1_455 1_455 ?
O5A OW2 O1 89.7(3) . 1_455 ?
O6B OW2 OW1 108.1(7) . 1_454 ?
O6A OW2 OW1 98.3(6) 1_455 1_454 ?
NA1 OW2 OW1 128.8(2) 2_556 1_454 ?
NA1 OW2 OW1 128.8(2) 3_556 1_454 ?
O5B OW2 OW1 62.4(3) 1_455 1_454 ?
S2B OW2 OW1 115.5(4) . 1_454 ?
S2A OW2 OW1 88.5(3) 1_455 1_454 ?
O5A OW2 OW1 92.4(4) . 1_454 ?
O1 OW2 OW1 177.8(4) 1_455 1_454 ?
O6B OW2 O4 81.1(5) . 3 ?
O6A OW2 O4 117.3(4) 1_455 3 ?
NA1 OW2 O4 156.1(5) 2_556 3 ?
NA1 OW2 O4 81.98(15) 3_556 3 ?
O5B OW2 O4 92.0(3) 1_455 3 ?
S2B OW2 O4 86.5(3) . 3 ?
S2A OW2 O4 110.7(3) 1_455 3 ?
O5A OW2 O4 69.9(2) . 3 ?
O1 OW2 O4 130.6(2) 1_455 3 ?
OW1 OW2 O4 50.46(16) 1_454 3 ?
O6B OW2 O4 81.1(5) . 2 ?
O6A OW2 O4 117.3(4) 1_455 2 ?
NA1 OW2 O4 81.98(15) 2_556 2 ?
NA1 OW2 O4 156.1(5) 3_556 2 ?
O5B OW2 O4 92.0(3) 1_455 2 ?
S2B OW2 O4 86.5(3) . 2 ?
S2A OW2 O4 110.7(3) 1_455 2 ?
O5A OW2 O4 69.9(2) . 2 ?
O1 OW2 O4 130.6(2) 1_455 2 ?
OW1 OW2 O4 50.46(16) 1_454 2 ?
O4 OW2 O4 85.1(3) 3 2 ?
 
_refine_diff_density_max    2.043
_refine_diff_density_min   -0.716
_refine_diff_density_rms    0.148



